Effect of rolling conditions on ferrite refinement of low-carbon steel
Refinement of the ferrite grains provides a promising approach to simultaneously improving both the strength and the toughness of steels. Among recent techniques to obtain ultrafine ferrite, dynamic strain induced transformation (DSIT) is used. This type of treatment is sensitive to steel composition, deformation temperature, the prior austenite grain size, strain and cooling rate. This work is aiming to improve the mechanical properties of steels using ferrite grain refining through trials on industrial scale using a compact strip production plant (CSP) with hot strip mill (HSM) containing six stands F1-F6 in EZDK Steel Company. The chemical composition of the trials was C (~0.046), Si (0.073) Mn (0.50) and Ti (0.008). The effect of final deformation temperature of 750, 775, 800 and 815°C on the microstructure and mechanical properties was studied. In addition the effect of strain rate variation at the final two rolling stands was correlated with the ferrite refining mechanisms. The ferrite grain size attained after refining varies from 10 μm to be 6 μm. Yield and tensile strength increased slightly through changing deformation temperature, with the advantage of keeping almost the original high ductility. Toughness of the processed steel increased with ferrite grain refining.
The production of ultrafine ferrite in low-carbon steel by strain-induced transformation
An investigation into the production of ultrafine (1 µm) equiaxed ferrite (UFF) grains in low-carbon steel was made using laboratory rolling, compression dilatometry, and hot torsion techniques. It was found that the hot rolling of thin strip, with a combination of high shear strain and high undercooling, provided the conditions most suitable for the formation of this type of microstructure. Although high strains could be applied in compression and torsion experiments, large volume fractions of UFF were not observed in those samples, possibly due to the lower level of undercooling achieved. It is thought that ferrite refinement was due to a strain-induced transformation process, and that ferrite grains nucleated on parallel and linear deformation bands that traversed austenite grains. These bands formed during the deformation process, and the undercooling provided by the contact between the strip and the work rolls was sufficient to drive the transformation to homogeneous UFF grains.
Importance of deformation induced ferrite and factors which control its formation
AbstractThe influence of strain, strain rate, temperature, and grain size on the formation of deformation induced ferrite has been examined. Deformation induced ferrite forms very readily in both fine and coarse grained steels and much more rapidly than the ferrite from strain free austenite. Very small strains are sufficient to induce the production of such ferrite and the temperature range over which it appears spans from just below the Ae3 temperature down to the undeformed Ar3 temperature. Although it forms readily in both coarse and fine grained steels, the volume fraction produced is sensitive to the austenite grain size. In coarse grained steels, deformation at low strain rates is concentrated along the grain faces; extensive dynamic recovery occurs, which is why the ferrite remains soft, so that only thin ferrite films are able to form. At higher strain rates, work hardening takes place so that the strength of the ferrite at high strains approaches that of the austenite. Under these conditions, th...